# ความต้านทานไฟฟ้าของธาตุ (หน้าข้อมูล)
ความต้านทานไฟฟ้า 
 T 80 K (-193 °C) 273 K (0 °C) 293 K (20 °C) 298 K (25 °C) 300 K (27 °C) 500 K (227 °C)  3 Li lithium use  10.0 nΩm  85.3 nΩm  92.8 nΩm  94.7 nΩm  95.5 nΩm  CRC (10-8 Ωm)  1.00  8.53  9.28  9.47  9.55  LNG (10-8 Ωm)    9.28    WEL (10-8 Ωm) (293 K-298 K) 9.4  4 Be beryllium use  0.75 nΩm  30.2 nΩm  35.6 nΩm  37.0 nΩm  37.6 nΩm  99 nΩm CRC (10-8 Ωm)  0.075  3.02  3.56  3.70  3.76  9.9 LNG (10-8 Ωm)    3.56    WEL (10-8 Ωm) (293 K-298 K) 4  5 B boron use    1.5×104 Ωm    LNG (10-8 Ωm)    1.5×1012    WEL (10-8 Ωm) (293 K-298 K) > 1012  6 C carbon (diamond) use  LNG (10-8 Ωm)    0.8 [sic]     6 C carbon (graphite) use  LNG (10-8 Ωm)    1375    WEL (10-8 Ωm) (293 K-298 K) about 1000 - direction dependent  11 Na sodium use  8.0 nΩm  43.3 nΩm  47.7 nΩm  48.8 nΩm  49.3 nΩm  CRC (10-8 Ωm)  0.80  4.33  4.77  4.88  4.93  LNG (10-8 Ωm)    4.77    WEL (10-8 Ωm) (293 K-298 K) 4.7  12 Mg magnesium use  5.57 nΩm  40.5 nΩm  43.9 nΩm  44.8 nΩm  45.1 nΩm  78.6 nΩm CRC (10-8 Ωm)  0.557  4.05  4.39  4.48  4.51  7.86 LNG (10-8 Ωm)    4.39    WEL (10-8 Ωm) (293 K-298 K) 4.4  13 Al aluminium use  2.45 nΩm  24.17 nΩm  26.50 nΩm  27.09 nΩm  27.33 nΩm  49.9 nΩm CRC (10-8 Ωm)  0.245  2.417  2.650  2.709  2.733  4.99 LNG (10-8 Ωm)    2.6548    WEL (10-8 Ωm) (293 K-298 K) 2.65  14 Si silicon use  LNG (10-8 Ωm)    105    WEL (10-8 Ωm) (293 K-298 K) about 100000  15 P phosphorus use  LNG (10-8 Ωm)    (white) 10 [sic]    WEL (10-8 Ωm) (293 K-298 K) 10  16 S sulfur use    (amorphous) 2×1015 Ωm    LNG (10-8 Ωm)    (amorphous) 2×1023    WEL (10-8 Ωm) (293 K-298 K) > 1023  17 Cl chlorine use    > 10 Ωm    LNG (10-8 Ωm)    >109    WEL (10-8 Ωm) (293 K-298 K) > 1010  19 K potassium use  13.4 nΩm  64.9 nΩm  72.0 nΩm  73.9 nΩm  74.7 nΩm  CRC (10-8 Ωm)  1.34  6.49  7.20  7.39  7.47  LNG (10-8 Ωm)    7.2    WEL (10-8 Ωm) (293 K-298 K) 7  20 Ca calcium use  6.5 nΩm  31.1 nΩm  33.6 nΩm  34.2 nΩm  34.5 nΩm  60. nΩm CRC (10-8 Ωm)  0.65  3.11  3.36  3.42  3.45  6.0 LNG (10-8 Ωm)    3.36    WEL (10-8 Ωm) (293 K-298 K) 3.4  21 Sc scandium use  (room temperature) (alpha, polycrystalline) calculated 562 nΩm CRC (10-8 Ωm) (290 K-300 K) 56.2 CR2 (10-8 Ωm) (room temperature) (alpha, amorphous) 70.9 CR2 (10-8 Ωm) (room temperature) (alpha, crystalline) 26.9 CR2 (10-8 Ωm) (room temperature) (alpha, polycrystalline) calculated from single crystal values 56.2 LNG (10-8 Ωm)    56.2    WEL (10-8 Ωm) (293 K-298 K) 55  22 Ti titanium use   0.39 µΩm  0.420 µΩm    CRC (10-8 Ωm)   39     LNG (10-8 Ωm)    42.0    WEL (10-8 Ωm) (293 K-298 K) 40  23 V vanadium use  24.1 nΩm  181 nΩm  197 nΩm  201 nΩm  202 nΩm  348 nΩm CRC (10-8 Ωm)  2.41  18.1  19.7  20.1  20.2  34.8 LNG (10-8 Ωm)    19.7    WEL (10-8 Ωm) (293 K-298 K) 20  24 Cr chromium use   118 nΩm  125 nΩm  126 nΩm  127 nΩm  201 nΩm CRC (10-8 Ωm)   11.8  12.5  12.6  12.7  20.1 LNG (10-8 Ωm)    12.5    WEL (10-8 Ωm) (293 K-298 K) 12.7  25 Mn manganese use  1.32 µΩm  1.43 µΩm  1.44 µΩm  1.44 µΩm  1.44 µΩm  1.49 µΩm CRC (10-8 Ωm)  132  143  144  144  144  149 LNG (10-8 Ωm)    144    WEL (10-8 Ωm) (293 K-298 K) 160  26 Fe iron use  6.93 nΩm  85.7 nΩm  96.1 nΩm  98.7 nΩm  99.8 nΩm  237 nΩm CRC (10-8 Ωm)  0.693  8.57  9.61  9.87  9.98  23.7 LNG (10-8 Ωm)    9.61    WEL (10-8 Ωm) (293 K-298 K) 9.7  27 Co cobalt use   56 nΩm  62.4 nΩm    CRC (10-8 Ωm)   5.6     LNG (10-8 Ωm)    6.24    WEL (10-8 Ωm) (293 K-298 K) 6  28 Ni nickel use  5.45 nΩm  61.6 nΩm  69.3 nΩm  71.2 nΩm  72.0 nΩm  177 nΩm CRC (10-8 Ωm)  0.545  6.16  6.93  7.12  7.20  17.7 LNG (10-8 Ωm)    6.93    WEL (10-8 Ωm) (293 K-298 K) 7  29 Cu copper use  2.15 nΩm  15.43 nΩm  16.78 nΩm  17.12 nΩm  17.25 nΩm  30.90 nΩm CRC (10-8 Ωm)  0.215  1.543  1.678  1.712  1.725  3.090 LNG (10-8 Ωm)    1.678    WEL (10-8 Ωm) (293 K-298 K) 1.7  30 Zn zinc use  11.5 nΩm  54.6 nΩm  59.0 nΩm  60.1 nΩm  60.6 nΩm  108.2 nΩm CRC (10-8 Ωm)  1.15  5.46  5.90  6.01  6.06  10.82 LNG (10-8 Ωm)    5.9    WEL (10-8 Ωm) (293 K-298 K) 5.9  31 Ga gallium use  CRC (10-8 Ωm)   13.6     LNG (10-8 Ωm) (30 °C) 25.795 WEL (10-8 Ωm) (293 K-298 K) 14  32 Ge germanium use LNG (10-8 Ωm)    53000    WEL (10-8 Ωm) (293 K-298 K) about 50000  33 As arsenic use    333 nΩm    LNG (10-8 Ωm)    33.3    WEL (10-8 Ωm) (293 K-298 K) 30  34 Se selenium use  LNG (10-8 Ωm)   (amorphous) 1.2 [sic]     WEL (10-8 Ωm) (293 K-298 K) high  35 Br bromine use    7.8×1010 Ωm    LNG (10-8 Ωm)    7.8×1018    WEL (10-8 Ωm) (293 K-298 K) > 1018  37 Rb rubidium use  26.5 nΩm  115 nΩm  128 nΩm  131 nΩm  133 nΩm  CRC (10-8 Ωm)  2.65  11.5  12.8  13.1  13.3  LNG (10-8 Ωm)    12.8    WEL (10-8 Ωm) (293 K-298 K) 12  38 Sr strontium use  36.4 nΩm  123 nΩm  132 nΩm  134 nΩm  135 nΩm  222 nΩm CRC (10-8 Ωm)  3.64  12.3  13.2  13.4  13.5  22.2 LNG (10-8 Ωm)    13.2    WEL (10-8 Ωm) (293 K-298 K) 13  39 Y yttrium use  (room temperature) (alpha, polycrystalline) 596 nΩm CRC (10-8 Ωm) (290 K-300 K) 59.6 CR2 (10-8 Ωm) (room temperature) (alpha, amorphous) 72.5 CR2 (10-8 Ωm) (room temperature) (alpha, crystalline) 35.5 CR2 (10-8 Ωm) (room temperature) (alpha, polycrystalline) 59.6 LNG (10-8 Ωm)    59.6    WEL (10-8 Ωm) (293 K-298 K) 56  40 Zr zirconium use  66.4 nΩm  388 nΩm  421 nΩm  429 nΩm  433 nΩm  765 nΩm CRC (10-8 Ωm)  6.64  38.8  42.1  42.9  43.3  76.5 LNG (10-8 Ωm)    42.1    WEL (10-8 Ωm) (293 K-298 K) 42  41 Nb niobium use   152 nΩm     CRC (10-8 Ωm)   15.2     LNG (10-8 Ωm)   15.2     WEL (10-8 Ωm) (293 K-298 K) 15  42 Mo molybdenum use  4.82 nΩm  48.5 nΩm  53.4 nΩm  54.7 nΩm  55.2 nΩm  106 nΩm CRC (10-8 Ωm)  0.482  4.85  5.34  5.47  5.52  10.6 LNG (10-8 Ωm)    5.34    WEL (10-8 Ωm) (293 K-298 K) 5  43 Tc technetium use  LNG (10-8 Ωm) (100 °C) 22.6 WEL (10-8 Ωm) (293 K-298 K) 20  44 Ru ruthenium use   71 nΩm     CRC (10-8 Ωm)   7.1     LNG (10-8 Ωm)   7.1     WEL (10-8 Ωm) (293 K-298 K) 7.1  45 Rh rhodium use   43.3 nΩm     CRC (10-8 Ωm)   4.3     LNG (10-8 Ωm)   4.33     WEL (10-8 Ωm) (293 K-298 K) 4.3  46 Pd palladium use  17.5 nΩm  97.8 nΩm  105.4 nΩm  107.3 nΩm  108.0 nΩm  179.4 nΩm CRC (10-8 Ωm)  1.75  9.78  10.54  10.73  10.80  17.94 LNG (10-8 Ωm)    10.54    WEL (10-8 Ωm) (293 K-298 K) 10  47 Ag silver use  2.89 nΩm  14.67 nΩm  15.87 nΩm  16.17 nΩm  16.29 nΩm  28.7 nΩm CRC (10-8 Ωm)  0.289  1.467  1.587  1.617  1.629  2.87 LNG (10-8 Ωm)    1.587    WEL (10-8 Ωm) (293 K-298 K) 1.6  48 Cd cadmium use   68 nΩm     use  (22 °C) 72.7 nΩm CRC (10-8 Ωm)   6.8     LNG (10-8 Ωm) (22 °C) 7.27 WEL (10-8 Ωm) (293 K-298 K) 7  49 In indium use   0.080 µΩm  83.7 nΩm    CRC (10-8 Ωm)   8.0     LNG (10-8 Ωm)    8.37    WEL (10-8 Ωm) (293 K-298 K) 8  50 Sn tin use   115 nΩm     CRC (10-8 Ωm)   11.5     LNG (10-8 Ωm)   11.5     WEL (10-8 Ωm) (293 K-298 K) 11  51 Sb antimony use   0.39 µΩm  417 nΩm    CRC (10-8 Ωm)   39     LNG (10-8 Ωm)    41.7    WEL (10-8 Ωm) (293 K-298 K) 40  52 Te tellurium use  LNG (10-8 Ωm)    (5.8-33)×103    WEL (10-8 Ωm) (293 K-298 K) about 10000  53 I iodine use   1.3×107 Ωm     LNG (10-8 Ωm)   1.3×1015     WEL (10-8 Ωm) (293 K-298 K) > 1015  55 Cs caesium use  41.6 nΩm  187 nΩm  205 nΩm  208 nΩm  210 nΩm  CRC (10-8 Ωm)  4.16  18.7  20.5  20.8  21.0  LNG (10-8 Ωm)    20.5    WEL (10-8 Ωm) (293 K-298 K) 20  56 Ba barium use  68.3 nΩm  302 nΩm  332 nΩm  0.340 µΩm  343 nΩm  724 nΩm CRC (10-8 Ωm)  6.83  30.2  33.2  34.0  34.3  72.4 LNG (10-8 Ωm)    33.2    WEL (10-8 Ωm) (293 K-298 K) 35  57 La lanthanum use  (room temperature) (alpha, polycrystalline) 615 nΩm CRC (10-8 Ωm) (290 K-300 K) 61.5 CR2 (10-8 Ωm) (room temperature) (alpha, polycrystalline) 61.5 LNG (10-8 Ωm)    61.5    WEL (10-8 Ωm) (293 K-298 K) 61  58 Ce cerium (beta, hex) use  (room temperature) (beta, polycrystalline) 828 nΩm CRC (10-8 Ωm) (beta, hex) (290 K-300 K) 82.8 CR2 (10-8 Ωm) (room temperature) (beta, polycrystalline) 82.8 LNG (10-8 Ωm)    (beta, hex) 82.8     58 Ce cerium (gamma, cubic) use  (room temperature) (gamma, polycrystalline) 744 nΩm CRC (10-8 Ωm)     74.4   CR2 (10-8 Ωm) (room temperature) (gamma, polycrystalline) 74.4 WEL (10-8 Ωm) (293 K-298 K) 74  59 Pr praseodymium use  (room temperature) (alpha, polycrystalline) 0.700 µΩm CRC (10-8 Ωm) (290 K-300 K) 70.0 CR2 (10-8 Ωm) (room temperature) (alpha, polycrystalline) 70.0 LNG (10-8 Ωm)    70.0    WEL (10-8 Ωm) (293 K-298 K) 70  60 Nd neodymium use  (room temperature) (alpha, polycrystalline) 643 nΩm CRC (10-8 Ωm) (290 K-300 K) 64.3 CR2 (10-8 Ωm) (room temperature) (alpha, polycrystalline) 64.3 LNG (10-8 Ωm)    64.3    WEL (10-8 Ωm) (293 K-298 K) 64  61 Pm promethium use  (room temperature) estimated 0.75 µΩm CRC (10-8 Ωm) (290 K-300 K) 75 est. CR2 (10-8 Ωm) (room temperature) (alpha, polycrystalline) 75 estimated LNG (10-8 Ωm)     64.0   WEL (10-8 Ωm) (293 K-298 K) 75  62 Sm samarium use  (room temperature) (alpha, polycrystalline) 0.940 µΩm CRC (10-8 Ωm) (290 K-300 K) 94.0 CR2 (10-8 Ωm) (room temperature) (alpha, polycrystalline) 94.0 LNG (10-8 Ωm)    94.0    WEL (10-8 Ωm) (293 K-298 K) 94  63 Eu europium use  (room temperature) (polycrystalline) 0.900 µΩm CRC (10-8 Ωm) (290 K-300 K) 90.0 CR2 (10-8 Ωm) (room temperature) (polycrystalline) 90.0 LNG (10-8 Ωm)    90.0    WEL (10-8 Ωm) (293 K-298 K) 90  64 Gd gadolinium use  (room temperature) (alpha, polycrystalline) 1.310 µΩm CRC (10-8 Ωm) (290 K-300 K) 131 CR2 (10-8 Ωm) (room temperature) (alpha, amorphous) 135.1 CR2 (10-8 Ωm) (room temperature) (alpha, crystalline) 121.7 CR2 (10-8 Ωm) (room temperature) (alpha, polycrystalline) 131.0 LNG (10-8 Ωm)    131    WEL (10-8 Ωm) (293 K-298 K) 130  65 Tb terbium use  (room temperature) (alpha, polycrystalline) 1.150 µΩm CRC (10-8 Ωm) (290 K-300 K) 115 CR2 (10-8 Ωm) (room temperature) (alpha, amorphous) 123.5 CR2 (10-8 Ωm) (room temperature) (alpha, crystalline) 101.5 CR2 (10-8 Ωm) (room temperature) (alpha, polycrystalline) 115.0 LNG (10-8 Ωm)    115    WEL (10-8 Ωm) (293 K-298 K) 120  66 Dy dysprosium use  (room temperature) (alpha, polycrystalline) 926 nΩm CRC (10-8 Ωm) (290 K-300 K) 92.6 CR2 (10-8 Ωm) (room temperature) (alpha, amorphous) 111.0 CR2 (10-8 Ωm) (room temperature) (alpha, crystalline) 76.6 CR2 (10-8 Ωm) (room temperature) (alpha, polycrystalline) 92.6 LNG (10-8 Ωm)    92.6    WEL (10-8 Ωm) (293 K-298 K) 91  67 Ho holmium use  (room temperature) (polycrystalline) 814 nΩm CRC (10-8 Ωm) (290 K-300 K) 81.4 CR2 (10-8 Ωm) (room temperature) (amorphous) 101.5 CR2 (10-8 Ωm) (room temperature) (crystalline) 60.5 CR2 (10-8 Ωm) (room temperature) (polycrystalline) 81.4 LNG (10-8 Ωm)    81.4    WEL (10-8 Ωm) (293 K-298 K) 94  68 Er erbium use  (room temperature) (polycrystalline) 0.860 µΩm CRC (10-8 Ωm) (290 K-300 K) 86.0 CR2 (10-8 Ωm) (room temperature) (amorphous) 94.5 CR2 (10-8 Ωm) (room temperature) (crystalline) 60.3 CR2 (10-8 Ωm) (room temperature) (polycrystalline) 86.0 LNG (10-8 Ωm)    86.0    WEL (10-8 Ωm) (293 K-298 K) 86  69 Tm thulium use  (room temperature) (polycrystalline) 676 nΩm CRC (10-8 Ωm) (290 K-300 K) 67.6 CR2 (10-8 Ωm) (room temperature) (amorphous) 88.0 CR2 (10-8 Ωm) (room temperature) (crystalline) 47.2 CR2 (10-8 Ωm) (room temperature) (polycrystalline) 67.6 LNG (10-8 Ωm)    67.6    WEL (10-8 Ωm) (293 K-298 K) 70  70 Yb ytterbium use  (room temperature) (beta, polycrystalline) 0.250 µΩm CRC (10-8 Ωm) (290 K-300 K) 25.0 CR2 (10-8 Ωm) (room temperature) (beta, polycrystalline) 25.0 LNG (10-8 Ωm)    25    WEL (10-8 Ωm) (293 K-298 K) 28  71 Lu lutetium use  (room temperature) (polycrystalline) 582 nΩm CRC (10-8 Ωm) (290 K-300 K) 58.2 CR2 (10-8 Ωm) (room temperature) (amorphous) 76.6 CR2 (10-8 Ωm) (room temperature) (crystalline) 34.7 CR2 (10-8 Ωm) (room temperature) (polycrystalline) 58.2 LNG (10-8 Ωm)    58.2    WEL (10-8 Ωm) (293 K-298 K) 56  72 Hf hafnium use  67.5 nΩm  304 nΩm  331 nΩm  337 nΩm  0.340 µΩm  631 nΩm CRC (10-8 Ωm)  6.75  30.4  33.1  33.7  34.0  63.1 LNG (10-8 Ωm)    33.1    WEL (10-8 Ωm) (293 K-298 K) 30  73 Ta tantalum use  26.2 nΩm  122 nΩm  131 nΩm  134 nΩm  135 nΩm  229 nΩm CRC (10-8 Ωm)  2.62  12.2  13.1  13.4  13.5  22.9 LNG (10-8 Ωm)    13.5    WEL (10-8 Ωm) (293 K-298 K) 13  74 W tungsten use  6.06 nΩm  48.2 nΩm  52.8 nΩm  53.9 nΩm  54.4 nΩm  103 nΩm CRC (10-8 Ωm)  0.606  4.82  5.28  5.39  5.44  10.3 LNG (10-8 Ωm)    5.28    WEL (10-8 Ωm) (293 K-298 K) 5  75 Re rhenium use   172 nΩm  193 nΩm    CRC (10-8 Ωm)   17.2     LNG (10-8 Ωm)    19.3    WEL (10-8 Ωm) (293 K-298 K) 18  76 Os osmium use   81.2 nΩm     CRC (10-8 Ωm)   8.1     LNG (10-8 Ωm)   8.12     WEL (10-8 Ωm) (293 K-298 K) 8.1  77 Ir iridium use   47 nΩm  47.1 nΩm    CRC (10-8 Ωm)   4.7     LNG (10-8 Ωm)    4.71    WEL (10-8 Ωm) (293 K-298 K) 4.7  78 Pt platinum use  19.22 nΩm  96 nΩm  105 nΩm  107 nΩm  108 nΩm  183 nΩm CRC (10-8 Ωm)  1.922  9.6  10.5  10.7  10.8  18.3 LNG (10-8 Ωm)    10.6    WEL (10-8 Ωm) (293 K-298 K) 10.6  79 Au gold use  4.81 nΩm  20.51 nΩm  22.14 nΩm  22.55 nΩm  22.71 nΩm  39.7 nΩm CRC (10-8 Ωm)  0.481  2.051  2.214  2.255  2.271  3.97 LNG (10-8 Ωm)    2.214    WEL (10-8 Ωm) (293 K-298 K) 2.2  80 Hg mercury use     961 nΩm   CRC (10-8 Ωm)     96.1   LNG (10-8 Ωm) (solid) 21 LNG (10-8 Ωm) (liquid) 95.8 WEL (10-8 Ωm) (293 K-298 K) 96  81 Tl thallium use   0.15 µΩm  0.18 µΩm    CRC (10-8 Ωm)   15     LNG (10-8 Ωm)    18    WEL (10-8 Ωm) (293 K-298 K) 15  82 Pb lead use  49 nΩm  192 nΩm  208 nΩm  211 nΩm  213 nΩm  383 nΩm CRC (10-8 Ωm)  4.9  19.2  20.8  21.1  21.3  38.3 LNG (10-8 Ωm)    20.8    WEL (10-8 Ωm) (293 K-298 K) 21  83 Bi bismuth use   1.07 µΩm  1.29 µΩm    CRC (10-8 Ωm)   107     LNG (10-8 Ωm)    129    WEL (10-8 Ωm) (293 K-298 K) 130  84 Po polonium use   (alpha) 0.40 µΩm     CRC (10-8 Ωm)   40     LNG (10-8 Ωm)   (alpha) 40.0     WEL (10-8 Ωm) (293 K-298 K) 43  88 Ra radium use    1 µΩm    LNG (10-8 Ωm)    100    WEL (10-8 Ωm) (293 K-298 K) 100  90 Th thorium use   147 nΩm     use  (22 °C) 15.4 CRC (10-8 Ωm)   14.7     LNG (10-8 Ωm) (22 °C) 15.4 WEL (10-8 Ωm) (293 K-298 K) 15  91 Pa protactinium use   177 nΩm     use  (22 °C) 19.1 CRC (10-8 Ωm)   17.7     LNG (10-8 Ωm) (22 °C) 19.1 WEL (10-8 Ωm) (293 K-298 K) 18  92 U uranium use   0.280 µΩm     CRC (10-8 Ωm)   28     LNG (10-8 Ωm)   28.0     WEL (10-8 Ωm) (293 K-298 K) 28  93 Np neptunium use  (22 °C) 1.220 µΩm LNG (10-8 Ωm) (22 °C) 122.0 WEL (10-8 Ωm) (293 K-298 K) 120  94 Pu plutonium use   1.460 µΩm     LNG (10-8 Ωm)   146.0     WEL (10-8 Ωm) (293 K-298 K) 150 T 80 K (-193 °C) 273 K (0 °C) 293 K (20 °C) 298 K (25 °C) 300 K (27 °C) 500 K (227 °C)